Physical properties and microstructure study of stainless steel 316L alloy fabricated by
selective laser melting
Nurul Kamariah Md Saiful Islam, Wan Sharuzi Wan Harun, Saiful Anwar Che Ghani, Mohd Asnawi Omar, Mohd Hazlen Ramli, and Muhammad Hussain Ismail
Citation: AIP Conference Proceedings 1901, 100015 (2017); View online: https://doi.org/10.1063/1.5010537
View Table of Contents: http://aip.scitation.org/toc/apc/1901/1 Published by the American Institute of Physics
Physical Properties and Microstructure Study of Stainless
Steel 316L Alloy Fabricated by Selective Laser Melting
Nurul Kamariah Md Saiful Islam1, b)
, Wan Sharuzi Wan Harun2, a)
Saiful Anwar Che Ghani2, c)
, Mohd Asnawi Omar3, d)
, Mohd Hazlen Ramli3, e)
Muhammad Hussain Ismail4, f)
1Institute of Postgraduate Studies, Universiti Malaysia Pahang, Lebuhraya Tun Razak, 26300 Gambang, Kuantan,
2Faculty of Mechanical Engineering, Universiti Malaysia Pahang, 26600 Pekan, Pahang, Malaysia. 3Additive Manufacturing Research and Innovation Center (AMRIC), KKTM Kuantan, KM8 Jalan Gambang, 25150
Kuantan, Pahang, Malaysia.
4Faculty of Mechanical Engineering Universiti Teknologi MARA, 40450 Shah Alam, Selangor, Malaysia. a) Corresponding author: email@example.com
b) firstname.lastname@example.org c) email@example.com d) firstname.lastname@example.org
e) email@example.com f) firstname.lastname@example.org
Abstract. Selective Laser Melting (SLM) demonstrates the 21st century’s manufacturing infrastructure in which powdered
raw material is melted by a high energy focused laser, and built up layer-by-layer until it forms three-dimensional metal parts. SLM process involves a variation of process parameters which affects the final material properties. 316L stainless steel compacts through the manipulation of building orientation and powder layer thickness parameters were manufactured by SLM. The effect of the manipulated parameters on the relative density and dimensional accuracy of the 316L stainless steel compacts, which were in the as-build condition, were experimented and analysed. The relationship between the microstructures and the physical properties of fabricated 316L stainless steel compacts was investigated in this study. The results revealed that 90° building orientation has higher relative density and dimensional accuracy than 0° building orientation. Building orientation was found to give more significant effect in terms of dimensional accuracy, and relative density of SLM compacts compare to build layer thickness. Nevertheless, the existence of large number and sizes of pores greatly influences the low performances of the density.
Selective Laser Melting (SLM) is one of the known additive manufacturing technology that utilises high energy focused laser to melt powdered raw material using a built up layer-by-layer techniques to form three-dimensional metal parts . Nevertheless, SLM true strength is the ability to allow manufacturing of bespoke part with complex geometries matching the properties of parts conventionally manufactured in series, for example, cast and cut . Despite this, to maximise the full potential of SLM, its particular issues need to be well understood.
Poor physical properties and residual porosity of the SLM manufactured parts prevent their usage for the application that requires high strength and fatigue resistance. Just like conventionally fabricated parts, properties of SLM parts do not rely only on microstructure but also on typically porous defects and their morphology, which are controlled by initial processing parameters . For this reason, most of the present-day studies have shown interest to understand how processing parameters affect microstructural evolution in SLM.
Due to the excellent corrosion resistance and properties exhibits by 316L stainless steel, this material has been chosen to be conducted by significant numbers of researches on SLM process [3-6]. Excellent physical properties such as dimensional accuracy and built part’s densification with 100 % relative density in practice arethechallenges for SLM process. In previous work, Yasa et al., (2011) has studied the effect of laser re-melting on the density of the built by SLM parts and managed to nearly reached 100 % of densification . Another research was done by Cherry et al., (2015) has introduced a semi-empirical formula of energy power density to improve the density of 316L stainless steel components. Layer thickness was designed as parts of the formula. Several studies were done to assess the effect of building direction on the mechanical properties of 316L stainless steel fabricated by SLM [9, 10].
This paper discusses the effect of building orientations and powder layer thickness of SLM process on the physical properties and microstructure of the SLM fabricated stainless steel 316L compacts using SLM, in the as-built condition. The dimensional accuracy, compact density and microstructure of the compacts are systematically discussed.
The metallic parts fabrication has been carried out using SLM machine SLM®125 HL (SLM Solutions, Germany). The 125 HL used an IPG-Faser laser with a power of 200 W. Stainless steel 316L powder utilised in this work was nitrogen gas-atomised powder with nominal chemical composition (wt.%) of 16–18 % Cr, 10.3 % Ni, 2.2 % Mo, 0.01 % C, 0.69 % Si, 0.99 % Mn, 0.02 % P, 0.005 % S and Fe balance.
Four sets of compacts were fabricated by SLM in the current study. The compacts were designed in the form of flat dog-bone shape with the dimension shown in Figure 1. The processing parameters are as listed in Table 1. Scanning speed and laser power were kept constant at 800 mm/s and 200 W, respectively. The manipulated parameters in this study are building orientation of 0° and 90°, and layer thickness of 30 and 50 μm.
The dimensional accuracy was measured on the as-built compacts at four main points which was the thickness of the compact, the largest width of the compact, width at the gauge and length of the compact. Digital Vernier calliper with 0.01 sensitivity, was employed. The compacts’ density was discovered by the Archimedes method using Precisa Gravimentrics equipment. In this method, the compacts’ density was calculated according to the Archimedes Principle. A compact's weight was measured in both distilled water and air. The compact’s density was gained when the distilled water’s density was given. The microstructures were observed under MEIJI-MT 7100 optical microscope (OM) at5x and 10x magnification.
TABLE 1. SLM parameters for the SS316L compacts fabrication
Compacts Laser Power (W) Scanning Speed (mm/s) Orientation (°) Building Layer Thickness (μm)
S01 200 800 0 30
S02 200 800 90 30
S03 200 800 0 50
S04 200 800 90 50
RESULTS AND DISCUSSION
Figure 2(a) reveals that 90° building orientation compacts have higher dimensional accuracy compare to 0° building orientation with 6.6 % differences. Meanwhile, 30 μm compacts show higher dimensional accuracy than 50 μm with only 0.5 % differences. The highest dimensional accuracy compact condition is 30 μm with 90° building orientation, while the lowest dimensional accuracy compact condition is 50 μm with 0° building orientation. From the result, it can be shown that the building layer thickness does not give significant effect on the dimensional accuracy of the compact as compared to building layer thickness. Despite this, all compact conditions can be saidto be above 90 % of dimensional accuracy.
The low dimensional accuracy of compacts can be related to the existence of remaining support at the bottom of compacts as illustrated in Figure 2(b). This was probably due to the poor quality of surface finish done at the lower part of the compacts during the post-process of removing compacts from the substrate. The remaining support, cause an addition in the measurement value of compact’s dimension. 0° building orientation compacts have a larger area of remaining support compare to 90° building orientation, thus, highly affect the value of the measurement.
The deformation of 0° building orientation compacts, as discussed, greatly influences the compact dimensional accuracy. The degree deformation as shown in Figure 2(c) indicates the changes in the actual dimension of the 0° building orientation compacts.
The trend in Figure 3 demonstrates that the 90° building orientation compacts have a higher relative density as compared to the 0° building orientation with 0.25 % differences. Meanwhile, the 50 μm layer thickness compacts have a higher relative density as compared to the 30 μmlayer thickness with 0.05 % differences. Compact condition that shows the highest relative density is 30 μm layer thickness with 90° building orientation compacts with the value of 99.2 % relative density. While the lowest relative density is 98.8 % relative density as shown by 50 μm layer thickness with 0° building orientation compacts.
Sun et al., (2016) mentioned in their paper that it is very challenging to reach SLM compact with a theoritical density of 100 % in practice . This is due to the possibilities of the existence of internal pores that were trapped within powders . Nevertheless, SLM is capable to fabricate a high density parts. This is supported by the result of the relative density gained in this study of between 99.2 % and 98.8 % whichindicate a high relative density of SLM compacts.
FIGURE 2. (a) Dimensional accuracy (%) for different condition of compacts; (b) Schematic diagrams showing the remaining
support (pink area) at the bottom of compacts (left) for 90q building orientation, and (right) for 0q building orientations; and (c) As-built compacts of 0q building orientation showing deformations occurred at the bottom surface of the compact.
FIGURE 3. Average relative density (%) of SLM compacts under different building orientations and powder layer thickness.
Figure 4 shows the inherent pores existed in the compact for 50 μm layer thickness with 0° building orientation condition, and 30 μm layer thickness with 90° building orientation condition, respectively. The finding provides evidence for limitation of the compact to reach 100 % fully dense. Figure 4(a) shows a larger size of pores as compared to Figure 4(b). The large size of pores causes the 50 μm layer thickness and 0º building orientation compact condition
30 μm/90° 50 μm/90° 30 μm/0° 50 μm/0° 99.08 98.76 93.83 93.24 98.9 99.2 98.8 99 30 μm/0° 30 μm/90° 50 μm/0° 50 μm/90°
to have the lowest density. This is in line with the finding by Sun et al., (2016) that the lowest density was due to the inherent pores trapped in the compacts .
FIGURE 4. Optical micrographs of pores of (a) as-build SLM processed 316L stainless steel powder with 50 μm layer thickness
and 0º building orientation, while b) is for 30 μm layer thickness and 90º building orientation.
The results reveal that 90° building orientation has higher dimensional accuracy than 0° building orientation. The low dimensional accuracy of the compact is due to large area of remaining support causing an additional measurement value of compact dimension and deformation. The same trend can be seen for relative density, where 90° building orientation shows higher relative density than 0° building orientation. Building orientation was found to give more significant effect in terms of dimensional accuracy and relative density of SLM compacts as compared to build layer thickness. The presence of large size of pores will significantly reduce the compact properties.
The authors would like to acknowledge the contributions of Universiti Malaysia Pahang (Grant no. RDU151314, RDU160354, GRS1503121), the Human Engineering Group (HEG), Universiti Malaysia Pahang and Kolej Kemahiran Tinggi Mara (KKTM) Kuantan for its comprehensive facilities support in this research.
1. F. Iacoviello, L. Reis, M. Fonte, M. Freitas, V. Infante, M. Seabra, J. Azevedo, A. Araújo, L. Reis, E. Pinto, N. Alves, R. Santos and J. Pedro Mortágua, Procedia Structural Integrity 1, 289-296 (2016).
2. H. Attar, M. Calin, L. C. Zhang, S. Scudino and J. Eckert, Materials Science and Engineering: A 593, 170-177 (2014).
3. P. Hanzl, M. Zetek, T. Bakša and T. Kroupa, Procedia Engineering 100, 1405-1413 (2015).
4. J. Čapek, M. Machová, M. Fousová, J. Kubásek, D. Vojtěch, J. Fojt, E. Jablonská, J. Lipov and T. Ruml,
Materials Science and Engineering: C 69, 631-639 (2016).
5. Z. Sun, X. Tan, S. B. Tor and W. Y. Yeong, Materials & Design 104, 197-204 (2016).
6. R. Casati, J. Lemke and M. Vedani, Journal of Materials Science & Technology 32 (8), 738-744 (2016). 7. E. Yasa and J. P. Kruth, Procedia Engineering 19, 389-395 (2011).
8. J. Cherry, H. Davies, S. Mehmood, N. Lavery, S. Brown and J. Sienz, The International Journal of Advanced Manufacturing Technology 76 (5-8), 869-879 (2015).
9. A. Mertens, S. Reginster, Q. Contrepois, T. Dormal, O. Lemaire and J. Lecomte-Beckers, presented at the Materials Science Forum, 2014 (unpublished).
10. W. Shifeng, L. Shuai, W. Qingsong, C. Yan, Z. Sheng and S. Yusheng, Journal of Materials Processing Technology 214 (11), 2660-2667 (2014).